Laser-induced change in the refractive index in some organic structures doped with nanoobjects. * The diffraction efficiency has not detected for these systems at this energy density. ** Dye TCNQ - 7,7,8,8,-tetracyanoquinodimethane – has been used in the paper .
It is well known that optoelectronics, telecommunication systems, aerospace, and correction of amplitude-phase aberration schemes, as well as laser, display, solar energy, gas storage and biomedicine techniques are searching for the new optical materials and for the new methods to optimize their properties. So many scientific and research groups are involving in this process and are opening the wide aspects of different applications of new materials, especially optical ones. It has been going on last century that simple manufacturing, design, ecology points of view, etc. indicate good advantage of the nanostructured materials with improved photorefractive parameters among other organic and inorganic systems.
Really, it should be tell that photorefractive properties change is correlated with the spectral, photoconductive and dynamics ones. The change in nonlinear refraction and cubic nonlinearity reveals the modification of barrier free electron pathway and dipole polarizability. From one side it is connected with the change of the dipole moment and the charge carrier mobility, from other side, it is regarded to the change of absorption cross section. Thus, this feature shows the unique place of photorefractive characteristics among other ones in order to characterize the spectral, photoconductive, photorefractive and dynamic properties of the optical materials.
It should be mentioned that promising nanoobjects, such as the fullerenes, the carbon nanotubes (CNTs), the quantum dots (QDs), the shungites, and the graphenes permit to found different area of applications of these nanoobjects [1-6]. The main reason to use the fullerenes, shungites, and quantum dots is connected with their unique energy levels and high value of electron affinity energy. The basic features of carbon nanotubes and graphenes are regarded to their high conductivity, strong hardness of their C-C bonds as well as complicated and unique mechanisms of charge carrier moving.
These peculiarities of carbon nanoobjects and their possible optoelectronics, solar energy, gas storage, medicine, display and biology applications connecting with dramatic improvement of photorefractive, spectral, photoconductive and dynamic parameters will be under consideration in this paper. In comparison with other effective nanoobjects the mail accent will be given namely on carbon nanotubes (CNTs) and their unique features to modify the properties of the optical materials.
The different experimental techniques have been used to study the properties of nanostructured materials.
To reveal the change of the photorefractive properties, as the systems under study the organic thin films based on conjugated monomer, polymer and liquid crystals sensitized with carbon nanotubes, fullerenes, shungites, graphenes oxides, or quantum dots have been chosen. Polyimides (PI), 2-cyclooctylamino-5-nitropyridine (COANP),
The nanostructured LC films have been placed onto glass substrates covered with transparent conducting layers based on ITO contacts. The nanostructured monomer or polymer solid films have been deposited on the substrate with ITO contact. For the electric measurements of volt-ampere parameters, gold contact has been put to the solid thin films upper side. The picture which can interpret the placement of the conducting contacts on the solid conjugated organic thin films is shown in Fig.2.
The bias voltage applied to the photosensitive polymer layers has been varied from 0 to 50 V. The current–voltage characteristics have been measured under the illumination conditions from dark to light. Voltmeter-electrometer В7—30 and Characteriscope—Z
The second harmonic of pulsed Nd-laser at wave length of 532 nm has been used. The laser energy density has been chosen in the range of 0.005-0.9 J×cm-2. The nanosecond laser regime with the pulse width of 10-20 ns has been applied. The amplitude-phase thin gratings have been recorded under Raman-Nath diffraction conditions according to which Λ-1 ≥
The spectral characteristics have been tested using Perkin Elmer lambda 9 spectrophotometer. Dynamic features of nanoobjects-doped LC films have been studied via the four-wave mixing technique and the Frederick’s scheme one. Atomic force microscopy (AFM) method using equipment of “NT-MDT” firm, “Bio47-Smena” in the “share-force” regime has been applied to analyze the diffraction relief into the solid conjugated nanostructured thin film.
3. Results and discussion
It should be noticed that previously, we demonstrated [5,6,8] the formation of barrier-free charge transfer pathways, increased dipole moment, and increased specific (per unit volume) local polarizability in some organic matrices doped with fullerenes, carbon nanotubes and quantum dots, where the formation of intermolecular complexes predominated over the intramolecular donor–acceptor interaction. The possible schemes of charge transfer between matrix organic molecule donor fragment and different efficient nanosensitizers including the additional graphene and shungites nanostructures are schematically shown in Fig. 4.
Analyzing the Fig.4, one can say that it is necessary to take into account that the charge transfer between matrix organic molecule donor fragment and nanasensitizers can be organized due to their high electron affinity energy (for example, electron affinity energy is close to 2 eV for shungites , to 2.65 eV for fullerenes [5,8] and to 3.8-4.2 eV for quantum dots ) that is more than the ones for intramolecular acceptor fragments (for example, electron affinity energy of COANP acceptor fragment is close to 0.54 eV  and to 1.14-1.4 eV for polyimide one ). Regarding graphenes it is necessary to take into account the high surface energy and planarity of the graphenes plane which can provoke to organize the charge transfer complex (CTC) with good advantage too. Regarding the CNTs it should be drawn the attention on the variety of charge transfer pathways, including those along and across a CNT, between CNTs, inside a multiwall CNT, between organic matrix molecules and CNTs, and between the donor and acceptor fragments of an organic matrix molecule.
It should be noticed that some supporting CTC results for PIs and COANP systems sensitized with nanoobjects can be presented via mass-spectrometry experiments. It is easy to show the organization of CTC using fullerenes acceptor. Really, the mass spectroscopy data point to the effective CTC formation between fullerene and donor part of PI (triphenylamine) and between fullerene and the HN group of COANP systems, respectively. For the 5 wt.% C70-COANP film, mass spectrometry curve contains two peaks. The first one at 400 C corresponds to the release rate of fragments with free fullerene masses. The second one is shifted to the temperature range of 520 °C and associated with the decomposition temperature of the fullerene-HN group complex. For the 0.5 wt.% C70-PI film, curve contains three peaks. The first one is observed also close to 400 C. The second peak is located at 560 °C and associated with the decomposition of fullerene- triphenylamine complex. It should be noticed that the melting temperature of these PIs is 700-1000 °C, thus, the third peak at the temperature higher 700 °C corresponds to the total decomposition of PI. Figure 5 presents the mass-spectrometry data.
By monitoring the diffraction response manifested in the laser scheme (see Fig.6); it is possible to study the dynamics of a photo-induced change in the refractive index of a sample and to calculate via  the nonlinear refraction and nonlinear third order optical susceptibility (cubic nonlinearity). An increase in the latter parameter characterizes a change in the specific (per unit volume) local polarizability and, hence, in the macroscopic polarization of the entire system.
The main results of this study are summarized in the Table 1 (Ref. 5,6,9,14-18) in comparison to the data of some previous investigations. An analysis of data presented in the Table 1 for various organic systems shows that the introduction of nanoobjects as active acceptors of electrons significantly influences the charge transfer under conditions where the intermolecular interaction predominates over the intramolecular donor–acceptor ones. Moreover, redistribution of the electron density during the recording of gratings in nanostructured materials changes the refractive index by at least one order of magnitude in comparision to that in the initial matrix. The diffusion of carriers from the bright to dark region during the laser recording of the interference pattern proceeds in three (rather than two) dimensions, which is manifested by a difference in the distribution of diffraction orders along the horizontal and vertical axes (see Fig.6). Thus, the grating displacement takes place in a three dimensional (3D) medium formed as a result of the nanostructirization (rather than in a 2D medium).
Some atomic force microscopy data are supported the realization of 3D-media via development of complicated diffraction relief into the solid thin conjugated films after transfer from the reversible regime to the irreversible one. Figure 7 demonstrates this fact. Two types of diffraction replica, namely due to interference of laser beams onto the thin films surface and due to the diffraction of these beams inside the body of the nanostructured media have been presented.
Using the obtained results, the nonlinear refraction
It was found that these parameters fall within
Moreover, it should be remained, that optical susceptibility χ(n), from fundamental point of view, directly connected with the dipole system polarizability (n) via equation (3) written in the paper :
where α(n) – dipole polarizability and υ – local volume.
Therefore, using the fact that polarizability of all structures can be accumulated from local volumes, it can be found that increased micropolarization of system (see eq.4) will predict the dynamic properties improvement and high electro-optical response speed.
It should be mentioned (see Table 1) that the larger nonlinear optical parameters have been found for CNTs-doped organic systems or CNTs-nanofibers-doped ones. It is natural to suggest (see Fig.8) that variations of the length, of the surface energy, of the angle of nanoobject orientation relative to the intramolecular donor can significantly change the pathway of charge carrier transfer, which will lead to changes in the electric field gradient, dipole moment (proportional to the product of charge and distance), and mobility of charge carriers.
In addition, the barrier free charge transfer will be influenced by competition between the diffusion and drift of carriers during the creation of diffraction patterns with various periods and, hence, differing charge localization at the grating nodes and antinodes. Indeed, in the case of a nanocomposite irradiated at small spatial frequencies (large periods of recorded grating), a drift mechanism of the carrier spreading in the electric field of an intense radiation field will moist probably predominate, while at large spatial frequencies (short periods of recorded grating) the dominating process is diffusion. This also naturally accounts for the aforementioned discrepancy of published data on photoinduced changes in the refractive index of nanocomposites, greater values of which were observed (see, e.g., data presented in the table for systems doped with CNTs and MIG nanofibers) at smaller spatial frequencies. Lower values of photoinduced changes in the refractive index of nanocomposites were observed at high spatial frequencies. This evidence predicts the strong correlations between photorefractive and photoconductive parameters.
To support the evidence on correlation between photorefractive and photoconductive features of the materials studied, the volt-current characteristics for nanoobjects-doped solid thin films and pure ones has been measured. After that charge carrier mobility has been estimated using the Child–Langmuir current–voltage relationship  following the formula (5) shown below:
For example, one can calculate the absolute values of the charge carrier mobility in pure and fullerene-modified PI samples. The results of these calculations show that the introduction of fullerenes leads to a tenfold increase in the mobility. The absolute values were estimated for a bias voltage of 10 V, a film thickness of
We have also calculated the relative values of the charge carrier mobility µ and estimated that two orders of magnitude differences of charge carrier mobility for the pure and nanoobjects-doped films has been found. Moreover, the following relation for the charge carrier mobility has been proposed:
The observation of the increase of charge carrier mobility, high refractive index and high value of cubic nonlinearities predicts that the nonlinear optical and the dynamic feature of the nanostructured conjugated materials can be optimized via nanostructurization with good advantage. It should be noted that classical inorganic nonlinear volume media (including BSO, LiNbO3, etc.) exhibit significantly lower nonlinearity, while bulk silicon based materials have nonlinear characteristics analogous to those of the organic thin film nanoobjects-doped materials under consideration.
|PI+malachite green dye||0.2||532||0.5-0.6||90-100||10-20||2.87x10-4|||
|PI+quantum dots based on CdSe(ZnS)||0.003||532||0.2-0.3||100||10||2.0x10-3|||
|PI + double-walled carbon nanotube powder||0.1||532||0.1||100||10||9.4x10-3|||
|PI + double-walled carbon nanotube powder||0.1||532||0.1||150||10||7.0x10-3|||
|PI+ mixture of CNT and nanofibers (type MIG)||0.1||532||0.3-0.6||90-100||10||11.7x10-3|||
|PI+ mixture of CNT and nanofibers (type MIG)||0.1||532||0.3-0.6||150||10||11.2x10-3|||
|Polymer-dispersed LC based on PI–C70 complex||0.2||532||0.1||90-100||10||1.2x 10-3|||
|COANP+ TCNQ**||0.1||676||2.2 Wсm-2||2x10-5|||
|Polymer-dispersed LC based on COANP–C70 complex||0.5||532||30×10−3||100||10||1.2×10-3||present|
|Polymer-dispersed LC based on COANP–C70 complex||5||532||17.5×10−3||100||20||1.4×10-3|||
|Polymer-dispersed LC based on COANP–nanotubes||0.1||532||30×10−3||100||10||2.8x10-3||present|
|Polymer-dispersed LC based on COANP–nanotubes||0.5||532||18.0×10−3||90-100||10-20||3.2x10-3|||
Thus, analysis of the obtained results leads to the following conclusions:
Doping with nanoobjects significantly influences the photorefractive properties of nanobjects-doped organic matrices. An increase in the electron affinity (cf. shungite, fullerenes, QDs) and specific area (cf. QDs, CNTs, nanofilers) implies a dominant role of the intermolecular processes leading to an increase in the dipole moment, local polarizability (per unit volume) of medium, and mobility of charge carriers.
A change in the distance between an intramolecular donor and intermolecular acceptor as a result of variation of the arrangement (rotation) of the introduced nanosensitizer leads to changes on the charge transfer pathway in the nanocomposite.
The variations of the length, of the surface energy, of the angle of nanoobject orientation relative to the intramolecular donor fragment of matrix organics can significantly change the pathway of charge carrier transfer, which will lead to changes in the electric field gradient and dipole moment.
Different values of nonlinear optical characteristics in systems with the same sensitizer type and concentration can be related to a competition between carrier drift and diffusion processes in a nanocomposite under the action of laser radiation.
Special role of the dipole moment as a macroscopic parameter of a medium accounts for a relationship between the photorefraction and the photoconductivity characteristics.
The photorefractive parameters change can be considered as the indicator of following dynamic and photoconductive characteristics change.
As the result of this discussion and investigation, new area of applications of the nanostructured materials can be found in the optoelectronics and laser optics, medicine, biology, telecommunications, display, microscopy technique, etc. Moreover, the nanostructured materials can be used for example, for development of 3D media with high density of recording information, as sensor in the gas storage and impurity testing, as photosensitive layer in the spatial light modulators, convertors, limiters, etc. devices.
The author would like to thank their Russian colleagues: Prof. N. M. Shmidt (Ioffe Physical-Technical Institute, St.-Petersburg, Russia), Prof. E.F.Sheka (University of Peoples’ Friendship, Moscow, Russia), Dr.N.N.Rozhkova (Institute of Geology, Karelian Research Centre, RAS), Dr.A.I.Plekhanov (Institute of Automation and Electrometry SB RAS, Novosibirsk, Russia), Dr.V.I.Studeonov and Dr.P.Ya.Vasilyev (Vavilov State Optical Institute, St.-Petersburg, Russia), as well as foreign colleagues: Prof. Francois Kajzar (Université d'Angers, Angers, France), Prof. D.P. Uskokovic (Institute of Technical Sciences of the Serbian Academy of Sciences and Arts, Belgrade, Serbia), Prof. I.Kityk (Politechnica Czestochowska, Czestochowa, Poland), Dr. R.Ferritto (Nanoinnova Technologies SL, Madrid, Spain) for their help in discussion and study at different their steps. The presented results are correlated with the work supported by Russian Foundation for Basic Researches (grant 10-03-00916, 2010-2012).
Couris S. Koudoumas E. Ruth A. A. Leach S. 1995 Concentration and wavelength dependence of the effective third-order susceptibility and optical limiting of C60 in toluene solution.
Robertson J. 2004 Realistic applications of CNTs.
Lee Wei Chen Hsu-Chih 2003 Diffraction efficiency of a holographic grating in a liquid-crystal cell composed of asymmetrically patterned electrodes.
Buchnev Oleksandr Dyadyusha Andriy Kaczmarek Malgosia Reshetnyak Victor Reznikov Yuriy 2007 Enhanced two-beam coupling in colloids of ferroelectric nanoparticles in liquid crystals.
Kamanina N. V. Emandi A. Kajzar F. Attias Andre´-Jean 2008 Laser-Induced Change in the Refractive Index in the Systems Based on Nanostructured Polyimide: Comparative Study with Other Photosensitive Structures.
Kamanina N. V. Serov S. V. Savinov V. P. Uskoković D. P. 2010 Photorefractive and photoconductive features of the nanostructured materials.
Kamanina N. V. Vasilenko N. A. 1997 Influence of operating conditions and of interface properties on dynamic characteristics of liquid-crystal spatial light modulators.
Kamanina N. V. 2005 Fullerene-dispersed liquid crystal structure: dynamic characteristics and self-organization processes.
Kamanina N. V. Serov S. V. Shurpo N. A. Rozhkova N. N. 2011 Photoinduced Changes in Refractive Index of Nanostructured Shungite-Containing Polyimide Systems.
Kamanina N. V. Shurpo N. A. Likhomanova S. V. Serov S. V. Ya P. Vasilyev V. G. Pogareva V. I. Studenov D. P. Uskokovic 2011 Influence of the Nanostructures on the Surface and Bulk Physical Properties of Materials.
Kamanina N. V. Plekhanov A. I. 2002 Mechanisms of optical limiting in fullerene-doped conjugated organic structures demonstrated with polyimide and COANP molecules.
Cherkasov Y. A. Kamanina N. V. Alexandrova E. L. Berendyaev V. I. Vasilenko N. A. Kotov B. V. 1998 Polyimides: New properties of xerographic, thermoplastic, and liquid-crystal structures.( SPIE International Symposium on Optical Science, Engineering and Instrumentation, San Diego, CA, USA, 1998)
Akhmanov S. A. Nikitin S. F. 1998 Physical Optics( Izdat. Mos. Gos. Univ., Moscow, 1998) [in Russian].
Kamanina N. V. Vasilyev Ya P. Serov S. V. Savinov V. P. Bogdanov. Yu K. Uskokovic D. P. 2010 Nanostructured Materials for Optoelectronic Applications.
Kamanina N. V. Serov S. V. Shurpo N. A. Likhomanova S. V. Timonin D. N. Kuzhakov P. V. Rozhkova N. N. Kityk I. V. Plucinski K. J. Uskokovic D. P. 2012 Polyimide-fullerene nanostructured materials for nonlinear optics and solar energy applications.
Ch Bosshard. Bosshard. K. Sutter P. Chapuis. Günter G. 1989 Linear- and nonlinear-optical properties of 2 -cyclooctylamino-5-nitropyridine.
Kamanina N. V. 2002 Optical investigations of a C70-doped 2-cyclooctylamino-5-nitropyridine-liquid crystal system.
Kamanina N. V. Uskokovic D. P. 2008 Refractive Index of Organic Systems Doped with Nano-Objects.
Chemla D. S. Eds. Zyss J. 1987 Nonlinear Optical Properties of Organic Molecules and Crystals 2( Orlando Academic Press, 1987), Translated into Russian, Moscow: Mir, 1989.
Gutman F. Lyons L. E. 1967 Organic Semiconductors Wiley New York
Mylnikov V. S. 1994in Advances in Polymer Science 115
Wang Y. Suna A. 1997 Fullerenes in Photoconductive Polymers. Charge Generation and Charge Transport.